Surface roughness (
In most of heterogeneous systems consisting of solid material in liquid medium the phase interface exhibits an electrical charge. This charge can play an important role in stability of these systems and in their behaviour in liquid surrounding. The knowledge of this behaviour is necessary for next usage of these materials. The electrical charge at solid-liquid interface is a key parameter for surface science and engineering. When the surface is charged, then it can attract ions of opposite charge (counter-ions) from the liquid. In this way the electrical double layer is created, consisting of two oppositely charged layers. Between the surface and volume liquid phase is a potential gradient and the potential of volume liquid phase is equal to zero. When the liquid flows along the solid surface, the electrical double layer divides. Inner layer (the solid phase) does not move, and adsorbed or bonded counter ions, while the outer layer flows along. The potential created between solid surface and this mobile interface is known as an electrokinetic potential or zeta potential (
Dissociation of the surface groups is a common charging mechanism in the case of latex particles, which are frequently used in biomedical applications . The adsorption of hydroxide ions created by enhanced autolysis of water at hydrophobic surfaces may be the reason for the hitherto unexplained charge of hydrophobic micro-fluidic substrates [2-4]. The behavior at hydrophobic and hydrophilic polymer surfaces is quite different. While on hydrophobic surface the surfactants displace water from the solid surface, it cannot displace water from the hydrophilic surface. In that case adsorption occurs mainly by electrostatic interactions between the surfactant “head” group and the surface groups . Pristine polymers exhibit the first (polymers without any functional groups on surface) or the third (when surface presents any functional groups able to dissociate in liquid) type of mechanisms depending on their surface chemistry. When polymers are deposited by metal nanostructures, the accumulation of electrons begins to play a role.
Zeta potential is a characteristic parameter for description of solid surface chemistry. It is an important physico-chemical property of cellulose , glass, metals, textile fabrics [7,8], wafers, ceramics , etc., giving information about chemistry, polarity, swelling, porosity and other surface characteristics. Zeta potential is used for characterization of natural and synthetic fibres and in investigation of their hydrophilicity, which is important for their interactions with dyes and surfactants [5,6,8]. It is also important for research of membranes, filters [10,11], pristine polymers [12-15] or polymers modified by plasma [12,15-18], by laser or by chemical coatings, e.g. by chitosan , biphenyldithiol , polyethyleneglycol  or by gold coatings [14,17]. It can also be used in research of textiles, where
Our team provides the study of different polymer foils and especially their variable modification for consequent usage in optics, electronics, tissue engineering, etc. For description and characterization of surface properties and their changes we apply a wide variety of analyses, such as X-ray photoelectron spectroscopy (XPS), atomic force microscopy (AFM), goniometry, infrared spectroscopy (IR), sheet resistance,
Zeta potential was determined for many polymer foils at constant pH value and also in the pH range for an isoelectric point study (zeta potential equals to zero). Polymer foils were than exposed to plasma, laser, gold sputtering and different chemical grafting. Changes of zeta potential values help us quickly recognize the chemical changes on modified surfaces due to different behaviour of surfaces in liquid surrounding. Polymer foils were modified in variable ways: by (i) plasma treatment, (ii) laser exposure, (iii) gold sputtering and consequent annealing, (iv) polyethylene glycol grafting, (v) dithiols grafting, (vi) cysteamine grafting, (vii) subsequent Au nanoparticles grafting, etc. All zeta potential results indicating different changes were subsequently confronted with other surfaces analyses.
2. Zeta potential determination
The zeta potential of planar samples represents the surface behaviour which occurs in the presence of an aqueous solution. It gives information about the nature and dissociation of reactive (functional) groups, about polarity, hydrophilicity or hydrophobicity of the solid surface, indirectly the chemical nature of studied sample and about ion or water sorption too [7,32]. This information is important for other polymer foils usage. Zeta potential can be determined using electrokinetic measurements, inclusive electrophoresis, sedimentation potential, electroosmosis, streaming current or streaming potential [7,24,30-35]. Measurements using multiple techniques are invaluable, since the errors with different techniques are often of opposite sign . The more detailed research and comparison of different techniques was presented previously . Most suitable for the planar samples is the streaming current or streaming potential approach [8,24,30,32,36,37]. Streaming current or streaming potential is generated by pressure-driven flow through a conduit . It is accomplished by applying a pressure, and the potential is induced as a result [24,35]. The zeta potential derived from the streaming potential or the streaming current is considered as
Streaming potential, streaming current and Helmholtz-Smoluchowski equation approach is correct and valid when electrolyte solution is forced through a narrow slit formed by two similar measured surfaces. This ensures that the thickness of the electrochemical double layer of the studied surface is smaller than the slit width and an overlapping of the double layers can be excluded [8,35].
While the determination of
Zeta potential depends on many solution and substrate parameters, such as pH, counter-ions concentration, valence and size, temperature, substrate material and its surface properties, etc. [30,31]. Strong effect on the
The study of pH effect has been accomplished by some investigators. Some of them find a linear variation with pH, while others reported a plateau at some pH values . Therefore we studied zeta potential of polymers at constant pH, only for isoelectric point determination we provided pH dependence. Also the effect of temperature should not be neglected, e.g. the
Zeta potential of polymer foils is also strongly affected by their surface roughness and other surface properties [13,32]. The roughness leads to geometry-induced changes, which can affect an electroosmotic flow and
Because of strong dependence of the measured values on experimental conditions discussed above, it is strongly recommended that all data on
We study zeta potential of several densities of polymer foils. Therefore zeta potential depends on counter-ion type and valence, but these effects do not play a role in the case of potassium and sodium counter-ion and observed differences are small for all polymer substrates , we finally used only potassium ions. The standard electrolyte was 0.00l mol/dm3 solution of KCl. The low electrolyte concentration ensures high sensitivity of the method [30,31,34]. To investigate the influence of electrolyte type and concentrations on
The following polymers in form of foils were used in this study (supplied by Goodfellow Ltd., UK): low density polyethylene (LDPE, density 0.92 g/cm3 in the form of 30 µm thick foils), biaxially oriented polyethyleneterephthalate (PET, density 1.3 g/cm3, 50 µm), polytetrafluoroethylene (PTFE, density 2.2 g/cm3, of three thicknesses 100, 50 and 25 µm), biaxially oriented polystyrene (PS, density 1.05 g/cm3, 30 µm), polypropylene (PP, density 0.9 g/cm3, 50 µm), polyamides (PA6 and PA66, both of them 40 µm), poly L-lactic acid (PLLA, density 1.25 g/cm3, 50 µm), polymethylpentene (PMP, density 0.84 g/cm3, 50 µm), polyimides (Upilex R, Upilex S and Kapton, all of them 50 µm), polyaramide (PAr, 10 µm), polybutylenterephthalate (PBT, 25 µm), poly(ethylene-2,6-naphthalene) (PEN, 7 µm), polymethylmetacrylate (PMMA, 7 µm), polycarbonate (PC, 2 mm). Oriented high density polyethylene (HDPE, density 0.952 g/cm3, 40 µm, supplied by Granitol Ltd., Czech Republic); polytetrafluoroethylene with perfluorovinyl pendant side chains ended by sulfonic acid groups (Nafion, total acid capacity: 0.95 to 1.01 meq/g, density 1.97 g/cm3, 173 µm, manufacturer DuPont, USA).
Polymer foils were studied in pristine form and also after modifications in the following variable ways: (i) plasma treatment, (ii) laser exposure, (iii) gold sputtering and consequent annealing, (iv) polyethylene glycol grafting, (v) dithiols grafting, (vi) methanol, dithiol and cysteamine grafting, (vii) steps (iv)-(vi) were supplemented by the subsequent Au nanoparticles/nanorods grafting.
2.3.1. Plasma treatment
Plasma treatment was performed on Balzers SCD 050 device under the following conditions: gas purity was 99.997%, flow rate 0.3 l/s, pressure 10 Pa, electrode distance 50 mm and its area 48 cm2, chamber volume approx. 1000 cm3, plasma volume 240 cm3. Exposure times differ for individual tested polymer foils and individual consequent modifications from 15 to 500 s, discharge power was 3.8 or 8.3 W and the treatment was accomplished at room temperature .
2.3.2. Laser irradiation
For laser irradiation of samples we employed the F2 laser (Lambda Physik LPF 202, wavelength of 157 nm, pulse duration of 15 ns). For the irradiation with the F2 laser, the light was polarized linearly with a MgF2 prism. For homogeneous illumination of the samples, we used only the central part of the beam profile by means of an aperture (10 mm - 3.5 mm). We performed the irradiation at fluences well below the ablation threshold of PET at 157 nm (29.6 mJ/cm2). The samples were mounted onto a translation stage and scanned at a speed of 14 mm/s. At a repetition rate of the laser of 11 Hz. We carried out the experiments in a flow box purged with nitrogen at a pressure of 110 kPa .
2.3.3. Gold sputtering and subsequent annealing
We deposited the gold nanostructures or nanolayers from a gold target (99.999%) by diode sputtering (BAL-TEC SCD 050 equipment) onto pristine polymers. The deposition was performed at room deposition temperature with a different deposition time and a current of 20 mA.
Post-deposition annealing of Au-covered PTFE was carried out in air at 300°C (± 3°C) for 1 h using a thermostat Binder oven. The heating rate was 5°C/min and the annealed samples were left to cool in air to room temperature (RT) .
2.3.4. Polyethylene glycol grafting
Polymers (PE and PS) were used for modification in Ar+ plasma discharge on a Balzers SCD 050 device. Immediately after the plasma treatment, plasma activated polymers were grafted by immersion into an aqueous solution (24 hours, room temperature, 2 wt.%) of polyethylene glycol (PEG, molecular weights (
2.3.5. Dithiols grafting and subsequent gold nanoparticles grafting
The plasma activated surface of PTFE was firstly grafted from methanol solution of biphenyl-4,4´-dithiol (BFD), 24 hours, room temperature, concentration 4 10-3 mol/dm3). Same samples was put in the colloidal solution of Au nanoparticles (24 hours, concentration 2.75 10-9 mol/dm3, size of nanoparticles was ca 15 nm . This solution was prepared by citrate reduction of K[AuCl4] . The non-bound chemicals were removed by immersion of the samples into distilled water for 24 hours .
2.3.6. Different thiols grafting and subsequent gold nanoobjects grafting
The samples were modified in direct (glow, diode) Ar+ plasma on Balzers SCD 050 device under the conditions presented in 2.3.1. Immediately after the plasma treatment the samples were inserted into water solution (2 wt. %) of 2-mercaptoethanol (ME), methanol solution (5.10-3 mol/dm3) of biphenyl-4,4'-dithiol (BPD) or into water solution (2 wt.%) of cysteamine (CYST) for 24 hours. To coat the polymers with the gold nanoobjects the plasma treated polymers with grafted thiols were immersed for 24 hours into freshly prepared colloidal citrate stabilized solution of Au nanoparticles (AuNPs), [44,46] or Au nanorods (AuNR), 0.1 mol/dm3 water solution of cetyltrimethylammonium bromide).
2.4. Diagnostic methods
2.4.1. Electrokinetic analysis
Zeta potential of all samples was determined by SurPASS Instrument (Anton Paar, Graz Austria). The SurPASS instrument is an electrokinetic analyzer for the investigation of the
The samples to be studied by streaming potential/current measurements have to be mechanically and chemically stable in the aqueous solutions used for the experiment. First, the geometry of the plug must be consolidated in the measuring cell. This can be checked by rinsing with the equilibrium liquid through repeatedly applying Δ
2.4.2. Contact angle
Contact angles of distilled water were measured at room temperature at two samples and at seven positions using a Surface Energy Evolution System (SEES, Masaryk University, Czech Republic). The „static“ contact angle was measured for all samples immediately after the plasma treatment (<10 min delay). Drops of 8.0±0.2 µl volume were deposited using automatic pipette (Transferpette Electronic Brand, Germany) and their images were taken with 5 s delay. Then the contact angles were evaluated using SEES code [12,13].
2.4.3. Surface roughness and morphology
The surface morphology and surface roughness
2.4.4. X-ray photoelectron spectroscopy
Concentrations of individual elements (O, C, F, N, Au and S) in the pristine and modified surface layer was measured by X-ray photoelectron spectroscopy (XPS). Omicron Nanotechnology ESCAProbeP spectrometer was used to measure photoelectron spectra (error of 10%). Exposed and analyzed area had dimension 2x3 mm2. X-ray source was monochromated at 1486.7 eV with step size 0.05 event. The spectra evaluation was carried out by CasaXPS programme .
2.4.5. Sheet resistance
Electrical sheet resistance (
2.4.6. Infrared spectroscopy
In some cases the changes of chemical structure were examined by Fourier Transform Infrared Spectroscopy (FTIR) on Bruker ISF 66/V spectrometer equipped with a Hyperion microscope with ATR (Ge) objective.
3.1. Pristine polymers
Firstly, it is evident
Fig. 1 shows that most of studied polymers are thought to be chemically inert, without reactive surface groups and displaying negative
Zeta potential of polymer foils is strongly affected by their surface roughness
We compare our results with those presented previously by other authors. As we mentioned above, many results cannot be compared in principle since the measurements were done using different techniques and quoted errors are often of opposite sign  or at different experimental conditions. Data on
Other comparison is difficult due to the authors examined the samples, combining polymer membrane foils, polymer fibres and colloidal dispersions for which the
Zeta potential values are often correlated with contact angle measurements and/or surface roughness determination. As we discussed previously, that is not correct in all cases . Most of polymers used in this study have no “reactive” surface groups in water solution and the surface charge only arises due to preferential adsorption of hydroxide ions in water solutions. The adsorption on the polymer surface is a drive force for
Zeta potential also serves for determination of isoelectric point (IEP), which is defined as the point at which the electrokinetic potential equals zero. It is also important characteristic for wrappers, for material for study of living cell adhesion, etc. Fig. 3 present zeta potential of several polymer foils as pH dependent. As it is clear, IEP of all polymer samples are obtained at pH ca 4. For this determination we have titrated samples by 0.1 mol/dm3 HCl in pH range from 7.0 to 2.5 .
3.2. Plasma and laser treatment of polymers
As it is known, plasma treatment affects the polymer surface to the depths from several hundred to several thousand angstroms but the bulk properties of polymers remain unchanged . Therefore only surface properties are changed dramatically by this treatment. Generally, during the plasma treatment the macromolecular chains are degraded, cleavaged and oxidized. Due to this, plasma treatment results in a dramatic increase of polymer wettability. The wettability increase is caused by creation of polar groups, exhibiting enhanced hydrophilicity, at the polymer surface . The similar effect on surface properties has also the laser irradiation . Fig. 4 shows the effect of plasma treatment (left) and laser irradiation (right) on zeta potential of selected polymer foils. For more transparent presentation only results obtained by streaming current method (eq. 1) are shown.
As it is clear from Fig. 4, plasma treatment results in a dramatic increase of the zeta-potential due to that the plasma modification of polymer surfaces leads to dramatic change of surface chemistry (e.g. chains and bonds scission, ablation, oxidation and cross-linking) and creation of polar groups . The effect of laser irradiation is not too strong due to that this treatment way influences surface chemistry and surface properties more weak [12,53]. Even in some causes zeta potential decreases after laser irradiation. It can be explained by the fact the cleavage of original bonds is most significant than surface oxidation after laser exposure in comparison with the plasma one. These effects strongly depend on plasma power or number of laser pulses.
For explanation of zeta potential behaviour on pristine and treated polymer surfaces we analysed surface chemistry by other techniques. Oxygen concentration in the surface layer of the laser modified polymers was determined from XPS spectra, the surface wettability and polarity were characterized by the measurement of contact angle of distilled water. These results are presented in Figs. 5 and 6. As it is clear form Fig. 5, after plasma or laser treatment increase the presence of oxygen groups on polymer surface. This increase in the oxygen content is much lower (Fig. 5, left) in comparison with that observed on the same polymers treated in plasma discharge (Fig. 5, right) [12,53].
Plasma treatment or laser irradiation result in a dramatic decline of the contact angle and corresponding increase of polymer wettability as it shown in Fig. 6. As is presented above, also contact angle analyses compare the result that laser irradiation effects surface chemistry and surface properties much less (Fig. 6, left) in comparison with plasma treatment (Fig. 6, right).
3.3. Gold sputtering and consequent annealing
In this part of work we have studied the changes of surface morphology and some other physico-chemical properties of sputtered gold nanostructures and nanolayers on polymer surface (PTFE) induced by post-deposition annealing . Fig. 7 presents zeta potential (left) and sheet resistance (right) of pristine PTFE (Fig. 7, thickness = 0) and Au coated PTFE in Au thicknesses dependences for room temperature (RT) and the same samples after annealing by different temperatures (100°C red line, 200°C green line, 300°C, blue line). Zeta potential was determined only for samples deposited by gold at RT and at 300°C.
We can see, that after deposition of metal layer zeta potential dramatically decrease due to increasing presence of surface coverage by metal and accompanying surface conductivity. For as-sputtered samples and very thin gold nanolayers, the zeta potential is close to that of pristine PTFE due to the discontinuous gold coverage since the PTFE surface plays dominant role in zeta potential value. Then, for thicker layers, where the gold coverage prevails over the original substrate surface, the zeta potential decreases rapidly and for the thicknesses above 20 nm remains nearly unchanged, indicating total coverage of original substrate by gold. For annealed samples, the dependence on the layer thickness is quite different. It is seen that the annealing leads to a significant increase of the zeta potential for thin nanolayers. This increase may be due to thermal degradation of the PTFE accompanied by production of excessive polar groups on the polymer surface, which plays the important role when the gold coverage is discontinuous .
These results on zeta potential are in good agreement with sheet resistance measurement and other surface analyses . As its obvious from Fig. 7 (right), for the as-sputtered samples the sheet resistance decreases rapidly in the narrow thickness from 10 to 15 nm when an electrical continuous gold coverage is formed. After annealing at 300°C a dramatic change in the resistance curve is observed. The annealed layers are electrically discontinuous up to the Au effective thickness of 70 nm above which the continuous coverage is created and a percolation limit is overcome. These results confirmed zeta potential analysis well as it is presented in Fig. 7, blue lines of both diagrams.
3.4. Polyethylene glycol grafting
As a representative of polymers grafted by polyethylene glycol we present PS grafted by polyethylene glycol (PEG) of different molecular weight 300 (PEG 300), 6000 (PEG 6000) and 20000 (PEG 20000) g/mol in Fig. 8. Modification of polymer surface by PEG plays important role in research of living cell adhesion and proliferation. Due to improving grafting process of PEG on PS it is better to treated polymer surface by plasma. We exposed PS surface by plasma for 50, 100 and 300 s and subsequently we grafted these surfaces by PEGs of mentioned molecular weights. These results have usage in tissue engineering due to positive effect to living cell adhesion and proliferation discussed below in Fig. 9.
As it is clear from Fig. 8, plasma treatment leads to increase of zeta potential due to creation of more polar groups on surface and this effect depends on exposure time positively. Subsequent grafting of PEG influences surface chemistry dependently on its molecular weight. While PEG 300 and PEG 20000 in most cases causes a slight decrease of zeta potential, PEG 6000 for shorter exposure time causes increase of zeta potential. It indicates quite different surface chemistry and nevertheless these changes are quiet slight, they play important role in process of adhesion and proliferation of living cells (see Fig. 9).
Adhesion and proliferation of rat vascular smooth muscle cells (VSMC) were studied on the pristine, plasma modified and subsequently PEG grafted PE and PS samples. It is supposed that the PEG bonds to several positions on the same macromolecular chain, limits chain mobility and in this way facilitates adsorption and colonization of the cells. Moreover, the oxygen-containing groups present in the PEG molecules might also enhance the colonization of the material by VSMCs as indicated by the highest final cell numbers on the PEG grafted PE observed on the 7th day after cell seeding .
Attractiveness of a substrate for cells is manifested not only by the number of growing VSMC cells but also by the homogeneity of their spreading over substrate surface. In Fig. 9 images of the cell cultures cultivated on PE and PS substrates subjected to different modification steps are shown. On pristine polymers the coverage with proliferating cells is not homogenous. It could be explained by the tendency of cells to compensate the insufficient cell-material adhesion by cell-to-cell adhesion, which leads to formation of cell clusters (aggregates) on the material surface. Plasma modification and especially the PEG grafting improves the coverage homogeneity substantially on both polymers.
3.5. Biphenyldithiol grafting and subsequent Au nanoparticles grafting
We tested several polymers (PE, PS, PET) for influence of surface properties affected by grafting of dithiols (methanol solution of biphenyl-4, 4´-dithiol (BFD) or 1, 2-ethanedithiol (ED)) and subsequent grafting by gold nanoparticles [42,54]. Before this grafting has also been polymer surface exposed to plasma discharge. As it is clear from Fig. 10 (left) for PET and BFD grafting, the zeta potential dramatically increases after plasma treatment due to creation of polar oxygen groups, which has been discussed above several times. The grafting of BFD leads to other zeta potential changes caused by thiol groups SH- bonded at polymer surface, which results in dissociation of this group in liquid surrounding during zeta potential measurement. This process leads to creation of negative charge on polymer surface and more presence of positive charge in electrolyte following by decrease of zeta potential. Subsequent Au nanoparticles grafting results to other decrease of zeta potential due to presence of metal gold nanostructures on polymer surface. From data obtained by both of methods and eqs. (1) and (2) (Fig. 10, left, HS, FM data resp.) it is clear the higher difference between HS and FM data for surface with Au nanoparticles which is caused by presence of some gold nanostrucrures and due to this increasing conductivity and also surface roughness.
In this case, the results on zeta potential were compared with infrared spectroscopy (Fig. 10, right), where the blue curve indicates the sulphur presence and the red curve indicates the gold presence in sample, confirming both of successful chemical graftings. FTIR spectroscopy was used for the characterization of chemical composition of modified PET samples. In the Fig. 10 (right) the differential FTIR spectra of the PET samples plasma treated and grafted in biphenyldithiol (BFD) and with Au nanoparticles are shown. The band at 790 cm-1 corresponds to absorption of the S-C group and the band at 761 cm-1 is assigned to the S-Au group. That is confirmation that both of graftings were successful as has been established by zeta potential analysis.
On the other hand, grafting of ED on PET was not successful. After the grafting of plasma treated PET with ED and Au nanoparticles the peak at 761 cm-1 (S-Au) in FTIR spectra was not detected. This finding supports the conclusion that no Au nanoparticles are bonded to the PET treated in ED .
3.6. Different thiols grafting and subsequent Au nanoobjects grafting
Other attempt to modify polymer surfaces was treatment of PET and PTFE by plasma discharge and subsequent grafting with different thiols (mercaptoethanol, ME, biphenyldithiol, BFD and cysteamine, CYST). Thiols are expected to be fixed via one of their functional groups –OH, –SH or –NH2 to reactive places created by the preceding plasma treatment. The remaining „free“ –SH group is then allowed to interact with gold nanoparticles or gold nanorods. The main goal of this study is to examine the effect of the plasma treatment and the thiol grafting on the binding of gold nanoobjects on the polymer surface. Chemical structure of the modified polymer films is expected to influence substantially theirs elektrokinetic potential in comparison with pristine polymers. Zeta potentials results for PET (left) and PTFE (right) modified by mentioned ways are presented in Fig. 11. Zeta potential of pristine PET, resp. PTFE, plasma treated PET, resp. PTFE, subsequently grafted with thiols and then with gold nanoobjects (nanoparticles, AuNP or nanorods, AuNR) are presented in Fig. 11. Zeta potential is affected by several factors, such as surface morphology, chemical composition (e.g. polarity, wetability) and electrical conductivity of surface. As it is clear from Fig. 11, zeta potential increases after plasma treatment. Due to higher ablation PTFE this increase is more significant at PET. After grafting of thiols in most cases zeta potential decreases due to presence of dissociative groups on surface. The Au nanoobjects grafting results in decrease of zeta potential values due to presence of gold nanostructures on surfaces.
Very interesting results we obtained after CYST exposition on PTFE, which results in dramatic increase of zeta potential. It can be explained by presence of “free” NH2- groups on surface caused probably by not preferential binding of cysteamine to plasma treated PTFE. This compound can be bonded probably not only via NH- group on activated surface but also via SH- group. This result was obtained only at PTFE, not at PET. At both of polymers the highest decrease of zeta potential after gold nanoobjects was found out after BPD grafting and subsequent grafting of Au nanoparticles.
Also in previous cases, zeta potential sensitively indicates all changes in surface chemistry and surface properties after any modification. These chemical changes were studied by XPS analysis. Elements (C(1s), O(1s), F (1s), S(2p), N (1s) and Au (4f)) concentrations (in at.%) determined by XPS measurements for PET and PTFE pristine and plasma treated (for 120 s) and grafted with (i) thiols (biphenyldithiol-BPD, cysteamine-CYST and mercaptoethanol-ME) and then (ii) grafted with Au nanoobjects (nanoparticles-AuNP and nanorods-AuNR) are presented in Table 2. The interesting results is for cysteamine on plasma treated PTFE, where nitrogen contents is not significantly different from the same sample of PET, but contents of bonded gold nanoparticles embody significantly lower value. It can confirm the zeta potential results discussed above. At both polymers obtained results clearly indicate the gold nanoparticles grafted at these substrates more easily than gold nanorods.
In our research all zeta potential values are always complemented with contact angle measurement by goniometry and determination of surface roughness and surface morphology by AFM, by spectroscopy analyses or other techniques.
Pristine polymer foils can be distinguished by electrokinetic analysis, as same as all modifications of polymer surface were indicated by changes in zeta potential. Due to this electrokinetic potential can serve as a fast and easy characteristic for study of changes in surface chemistry. Elektrokinetic analysis is the fast, the easy and very sensitive method for characterization solid substrates.
This work was supported by the grants of the GACR projects Nos. P108/10/1106, P108/12/1168 and P503/12/1424.